Successfully reported this slideshow.
Upcoming SlideShare
×

# Groover fundamentals-modern-manufacturing-4th-solution-manuel

204,316 views

Published on

• Full Name
Comment goes here.

Are you sure you want to Yes No

### Groover fundamentals-modern-manufacturing-4th-solution-manuel

1. 1. SOLUTION MANUAL
12. 12. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-02-09, 03-02-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 5 Flow Curve 3.4 In Problem 3.3, determine the strength coefficient and the strain-hardening exponent in the flow curve equation. Be sure not to use data after the point at which necking occurred. Solution: Starting volume of test specimen V = 125(62.5) = 7812.5 mm3 . Select two data points: (1) F = 23042 N and L = 131.25 mm; (2) F = 28913 N and L = 147.01 mm. (1) A = V/L = 7812.5/131.25 = 59.524 mm2 . Stress σ = 23042/59.524 = 387.1 MPa. Strain ε = ln(131.25/125) = 0.0488 (2) A = 7812.5/147.01 = 53.143 mm2 . Stress σ = 28913/53.143 = 544.1 MPa. Strain ε = ln(147.01/125) = 0.1622 Substituting these values into the flow curve equation, we have (1) 387.1 = K(0.0488)n and (2) 544.1 = K(0.1622)n 544.1/387.1 = (0.1622/0.0488)n 1.4056 = (3.3238)n ln(1.4056) = n ln(3.3238) 0.3405 = 1.2011 n n = 0.283 Substituting this value with the data back into the flow curve equation, we obtain the value of the strength coefficient K: K = 387.1/(0.0488).283 = 909.9 MPa K = 544.1/(0.1622).283 = 910.4 MPa Use average K = 910.2 MPa The flow curve equation is: σ = 910.2 ε0.283 3.5 In a tensile test on a metal specimen, true strain = 0.08 at a stress = 265 MPa. When true stress = 325 MPa, true strain = 0.27. Determine the strength coefficient and the strain-hardening exponent in the flow curve equation. Solution: (1) 265 = K(0.08)n and (2) 325 = K(0.27)n 325/265 = (0.27/0.08)n 1.2264 = (3.375)n n ln(3.375) = ln(1.2264) 1.2164 n = 0.2041 n = 0.1678 Substituting this value with the data back into the flow curve equation, we obtain the value of the strength coefficient K: (1) K = 265/(0.08).1678 = 404.85 MPa (2) K = 325/(0.27).1678 = 404.85 MPa The flow curve equation is: σ = 404.85 ε0.1678 3.6 During a tensile test, a metal has a true strain = 0.10 at a true stress = 37,000 lb/in2 . Later, at a true stress = 55,000 lb/in2 , true strain = 0.25. Determine the strength coefficient and strain-hardening exponent in the flow curve equation. Solution: (1) 37,000 = K(0.10)n and (2) 55,000 = K(0.25)n 55,000/37,000 = (0.25/0.10)n 1.4865 = (2.5)n n ln(2.5) = ln(1.4865) 0.9163 n = 0.3964 n = 0.4326 Substituting this value with the data back into the flow curve equation, we obtain the value of the strength coefficient K: (1) K = 37,000/(0.10)0.4326 = 100,191 lb/in2 (2) K = 55,000/(0.25)0.4326 = 100,191 lb/in2 The flow curve equation is: σ = 100,191 ε0.4326
13. 13. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-02-09, 03-02-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 6 3.7 In a tensile test a metal begins to neck at a true strain = 0.28 with a corresponding true stress = 345.0 MPa. Without knowing any more about the test, can you estimate the strength coefficient and the strain-hardening exponent in the flow curve equation? Solution: If we assume that n = ε when necking starts, then n = 0.28. Using this value in the flow curve equation, we have K = 345/(0.28).28 = 492.7 MPa The flow curve equation is: σ = 492.7 ε0.28 3.8 A tensile test for a certain metal provides flow curve parameters: strain-hardening exponent is 0.3 and strength coefficient is 600 MPa. Determine (a) the flow stress at a true strain = 1.0 and (b) true strain at a flow stress = 600 MPa. Solution: (a) Yf = 600(1.0).3 = 600 MPa (b) ε = (600/600)1/.3 = (1.0)3.33 = 1.00 3.9 The flow curve for a certain metal has a strain-hardening exponent of 0.22 and strength coefficient of 54,000 lb/in2 . Determine (a) the flow stress at a true strain = 0.45 and (b) the true strain at a flow stress = 40,000 lb/in2 . Solution: (a) Yf = 54,000(0.45).22 = 45,300 lb/in2 (b) ε = (40,000/54,000)1/.22 = (0.7407)4.545 = 0.256 3.10 A metal is deformed in a tension test into its plastic region. The starting specimen had a gage length = 2.0 in and an area = 0.50 in2 . At one point in the tensile test, the gage length = 2.5 in, and the corresponding engineering stress = 24,000 lb/in2 ; at another point in the test prior to necking, the gage length = 3.2 in, and the corresponding engineering stress = 28,000 lb/in2 . Determine the strength coefficient and the strain-hardening exponent for this metal. Solution: Starting volume V = LoAo = 2.0(0.5) = 1.0 in3 (1) A = V/L = 1.0/2.5 = 0.4 in2 So, true stress σ = 24,000(0.5)/0.4 = 31,250 lb/in2 and ε = ln(2.5/2.0) = 0.223 (2) A = 1.0/3.2 = 0.3125 in2 So, true stress σ = 28,000(0.5)/0.3125 = 44,800 lb/in2 and ε = ln(3.2/2.0) = 0.470 These are two data points with which to determine the parameters of the flow curve equation. (1) 31,250 = K(0.223)n and (2) 44,800 = K(0.470)n 44,800/31,250 = (0.470/0.223)n 1.4336 = (2.1076)n ln(1.4336) = n ln(2.1076) 0.3602 = .7455 n n = 0.483 (1) K = 31,250/(0.223).483 = 64,513 lb/in2 (2) K = 44,800/(0.470).483 = 64,516 lb/in2 Use average K = 64,515 lb/in2 The flow curve equation is: σ = 64,515 ε0.483 3.11 A tensile test specimen has a starting gage length = 75.0 mm. It is elongated during the test to a length = 110.0 mm before necking occurs. Determine (a) the engineering strain and (b) the true strain. (c) Compute and sum the engineering strains as the specimen elongates from: (1) 75.0 to 80.0 mm, (2) 80.0 to 85.0 mm, (3) 85.0 to 90.0 mm, (4) 90.0 to 95.0 mm, (5) 95.0 to 100.0 mm, (6) 100.0 to 105.0 mm, and (7) 105.0 to 110.0 mm. (d) Is the result closer to the answer to part (a) or part (b)? Does this help to show what is meant by the term true strain? Solution: (a) Engineering strain e = (110 - 75)/75 = 35/75 = 0.4667
14. 14. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-02-09, 03-02-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 7 (b) True strain ε = ln(110/75) = ln(1.4667) = 0.383 (c) (1) L = 75 to 80 mm: e = (80 - 75)/75 = 5/75 = 0.0667 (2) L = 80 to 85 mm: e = (85 - 80)/80 = 5/80 = 0.0625 (3) L = 85 to 90 mm: e = (90 - 85)/85 = 5/85 = 0.0588 (4) L = 90 to 95 mm: e = (95 - 90)/90 = 5/90 = 0.0556 (5) L = 95 to 100 mm: e = (100 - 95)/95 = 5/95 = 0.0526 (6) L = 100 to 105 mm: e = (105 - 100)/100 = 5/100 = 0.0500 (7) L = 105 to 110 mm: e = (110 - 105)/105 = 5/105 = 0.0476 _____________________________________________ Sum of incremental engineering strain values = 0.3938 (d) The resulting sum in (c) is close to the true strain value in (b). The summation process is an approximation of the integration over the range from 75 to 110 mm in (b). As the interval size is reduced, the summation becomes closer to the integration value. 3.12 A tensile specimen is elongated to twice its original length. Determine the engineering strain and true strain for this test. If the metal had been strained in compression, determine the final compressed length of the specimen such that (a) the engineering strain is equal to the same value as in tension (it will be negative value because of compression), and (b) the true strain would be equal to the same value as in tension (again, it will be negative value because of compression). Note that the answer to part (a) is an impossible result. True strain is therefore a better measure of strain during plastic deformation. Solution: Engineering strain e = (2.0 - 1.0)/1.0 = 1.0 True strain ε = ln(2.0/1.0) = ln(2.0) = 0.693 (a) To be compressed to the same engineering strain (e = -1.0) the final height of the compression specimen would have to be zero, which is impossible. (b) To be compressed to the same true strain value (e = -0.693) the final height of the compression specimen can be determined as follows: ε = -.693 = ln(Lf/Lo) Lf/Lo = exp.(-0.693) = 0.500 Therefore, Lf = 0.5 Lo 3.13 Derive an expression for true strain as a function of D and Do for a tensile test specimen of round cross section, where D = the instantaneous diameter of the specimen and Do is its original diameter. Solution: Starting with the definition of true strain as ε = ln(L/Lo) and assuming constant volume, we have V = AoLo = AL Therefore, L/Lo = Ao/A A = πD2 and Ao = πDo 2 Ao/A = πDo 2 /πD2 = (Do/D)2 ε = ln(Do/D)2 = 2 ln(Do/D) 3.14 Show that true strain = ln(1 + e), where e = engineering strain. Solution: Starting definitions: (1) ε = ln(L/Lo) and (2) e = (L - Lo)/Lo Consider definition (2): e = L/Lo - Lo/Lo = L/Lo - 1 Rearranging, 1 + e = L/Lo Substituting this into definition (1), ε = ln(1 + e) 3.15 Based on results of a tensile test, the flow curve strain-hardening exponent = 0.40 and strength coefficient = 551.6 MPa. Based on this information, calculate the (engineering) tensile strength for the metal.
15. 15. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-02-09, 03-02-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 8 Solution: Tensile strength occurs at maximum value of load. Necking begins immediately thereafter. At necking, n = ε. Therefore, σ = 551.6(0.4)0.4 = 382.3 MPa. This is a true stress. TS is defined as an engineering stress. From Problem 3.15, we know that ε = 2 ln(Do/D). Therefore, 0.4 = 2 ln(Do/D) ln(Do/D) = .4/2 = 0.2 Do/D = exp(0.2) = 1.221 Area ratio = (Do/D)2 = (1.221)2 = 1.4918 The ratio between true stress and engineering stress would be the same ratio. Therefore, TS = 1.4918(382.3) = 570.3 MPa 3.16 A copper wire of diameter 0.80 mm fails at an engineering stress = 248.2 MPa. Its ductility is measured as 75% reduction of area. Determine the true stress and true strain at failure. Solution: Area reduction AR = (Ao - Af)/Ao = 0.75 Ao - Af = 0.75 Ao Ao - 0.75Ao = 0.25 Ao = Af If engineering stress = 248.2 MPa, then true stress σ = 248.2/0.25 = 992.8 MPa True strain ε = ln(Lf/Lo) = ln(Ao/Af) = ln(4) = 1.386. However, it should be noted that these values are associated with the necked portion of the test specimen. 3.17 A steel tensile specimen with starting gage length = 2.0 in and cross-sectional area = 0.5 in2 reaches a maximum load of 37,000 lb. Its elongation at this point is 24%. Determine the true stress and true strain at this maximum load. Solution: Elongation = (L - Lo)/Lo = 0.24 L - Lo = 0.24 Lo L = 1.24 Lo A = Ao/1.24 = 0.8065 Ao True stress σ = 37,000/0.8065(0.5) = 91,754 lb/in2 True strain ε = ln(1.24) = 0.215 Compression 3.18 A metal alloy has been tested in a tensile test with the following results for the flow curve parameters: strength coefficient = 620.5 MPa and strain-hardening exponent = 0.26. The same metal is now tested in a compression test in which the starting height of the specimen = 62.5 mm and its diameter = 25 mm. Assuming that the cross section increases uniformly, determine the load required to compress the specimen to a height of (a) 50 mm and (b) 37.5 mm. Solution: Starting volume of test specimen V = πhDo 2 /4 = 62.5π(25)2 /4 = 30679.6 mm3 . (a) At h = 50 mm, ε = ln(62.5/50) = ln(1.25) = 0.223 Yf = 620.5(.223).26 = 420.1 MPa A = V/L = 30679.6/50 = 613.6 mm2 F = 420.1(613.6) = 257,770 N (b) At h = 37.5 mm, ε = ln(62.5/37.5) = ln(1.667) = 0.511 Yf = 620.5(0.511).26 = 521.1 MPa A = V/L = 30679.6 /37.5 = 818.1 mm2 F = 521.1(818.1) = 426,312 N 3.19 The flow curve parameters for a certain stainless steel are strength coefficient = 1100 MPa and strain- hardening exponent = 0.35. A cylindrical specimen of starting cross-sectional area = 1000 mm2 and height = 75 mm is compressed to a height of 58 mm. Determine the force required to achieve this compression, assuming that the cross section increases uniformly.
18. 18. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-02-09, 03-02-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 11 Viscosity of Fluids 3.28 Two flat plates, separated by a space of 4 mm, are moving relative to each other at a velocity of 5 m/sec. The space between them is occupied by a fluid of unknown viscosity. The motion of the plates is resisted by a shear stress of 10 Pa due to the viscosity of the fluid. Assuming that the velocity gradient of the fluid is constant, determine the coefficient of viscosity of the fluid. Solution: Shear rate = (5 m/s x 1000 mm/m)/(4 mm) = 1250 s-1 η = (10N/m2 )/(1250 s-1 ) = 0.008 N-s/m2 = 0.008 Pa-s 3.29 Two parallel surfaces, separated by a space of 0.5 in that is occupied by a fluid, are moving relative to each other at a velocity of 25 in/sec. The motion is resisted by a shear stress of 0.3 lb/in2 due to the viscosity of the fluid. If the velocity gradient in the space between the surfaces is constant, determine the viscosity of the fluid. Solution: Shear rate = (25 in/sec)/(0.5 in) = 50 sec-1 η = (0.3 lb/in2 )/(50 sec-1 ) = 0.0006 lb-sec/in2 . 3.30 A 125.0-mm-diameter shaft rotates inside a stationary bushing whose inside diameter = 125.6 mm and length = 50.0 mm. In the clearance between the shaft and the bushing is a lubricating oil whose viscosity = 0.14 Pa-s. The shaft rotates at a velocity of 400 rev/min; this speed and the action of the oil are sufficient to keep the shaft centered inside the bushing. Determine the magnitude of the torque due to viscosity that acts to resist the rotation of the shaft. Solution: Bushing internal bearing area A = π(125.6)2 x 50/4 = 19729.6 mm2 = 19729.2(10-6 ) m2 d = (125.6 - 125)/2 = 0.3 mm v = (125π mm/rev)(400 rev/min)(1 min/60 sec) = 2618.0 mm/s Shear rate = 2618/0.3 = 8726.6 s-1 τ = (0.14)(8726.6) = 1221.7 Pa = 1221.7 N/mm2 Force on surface between shaft and bushing = (1221.7 N/mm2 )(19729.2(10-6 )) = 24.1 N Torque T = 24.1 N x 125/2 mm = 1506.4 N-mm = 1.506 N-m
21. 21. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-03-09, 03-03-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 3 Problems 4.1 The starting diameter of a shaft is 25.00 mm. This shaft is to be inserted into a hole in an expansion fit assembly operation. To be readily inserted, the shaft must be reduced in diameter by cooling. Determine the temperature to which the shaft must be reduced from room temperature (20°C) in order to reduce its diameter to 24.98 mm. Refer to Table 4.1. Solution: For steel, α = 12(10-6 ) mm/mm/°C according to Table 4.1. Revise Eq. (4.1) to D2 - D1 = αD1 (T2 - T1). 24.98 - 25.00 = 12(10-6 )(25.00)(T2 - 20) -0.02 = 300(10-6 )(T2 - 20) -0.02 = 0.0003(T2 - 20) = 0.0003T2 - 0.006 -.02 + 0.006 = 0.0003T2 -0.014 = 0.0003T2 T2 = -46.67°C 4.2 A bridge built with steel girders is 500 m in length and 12 m in width. Expansion joints are provided to compensate for the change in length in the support girders as the temperature fluctuates. Each expansion joint can compensate for a maximum of 40 mm of change in length. From historical records it is estimated that the minimum and maximum temperatures in the region will be -35°C and 38°C, respectively. What is the minimum number of expansion joints required? Solution: Assume L1 =500 m at -35 C, α=12x10-6 /C L2 – L1 = αL1(T2 – T1) L2 – L1 = 12x10-6 (500)(38 – (-35)) L2 – L1 = 0.42 m Each expansion joint will control 40 mm = 0.04 m of expansion. 10 joints will provide 0.40 m of expansion. 11 joints will provide 0.45 m of expansion. Therefore, a minimum of 11 joints are needed for coverage of the total length. Each bridge section will be 500/11 = 45.5 m long. 4.3 Aluminum has a density of 2.70 g/cm3 at room temperature (20°C). Determine its density at 650°C, using data in Table 4.1 as a reference. Solution: Assume a 1 cm3 cube, 1 cm on each side. From Table 4.1, α = 24(10-6 ) mm/mm/°C L2 - L1 = αL1 (T2 - T2). L2 = 1.0 + 24(10-6 )(1.0)(650 - 20) = 1.01512 cm (L2 )3 = (1.01512)3 = 1.04605 cm3 Assume weight remains the same; thus ρ at 650°C = 2.70/1.04605 = 2.581 g/cm3 4.4 With reference to Table 4.1, determine the increase in length of a steel bar whose length = 10.0 in, if the bar is heated from room temperature of 70°F to 500°F. Solution: Increase = (6.7 x 10-6 in/in/F)(10.0 in)(500°F - 70°F) = 0.0288 in. 4.5 With reference to Table 4.2, determine the quantity of heat required to increase the temperature of an aluminum block that is 10 cm x 10 cm x 10 cm from room temperature (21°C) to 300°C. Solution. Heat = (0.21 cal/g-°C)(103 cm3 )(2.70 g/cm3 )(300°C - 21°C) = 158,193 cal. Conversion: 1.0 cal = 4.184J, so heat = 662,196 J. 4.6 What is the resistance R of a length of copper wire whose length = 10 m and whose diameter = 0.10 mm? Use Table 4.3 as a reference. Solution: R = rL/A, A = π(0.1)2 /4 = 0.007854 mm2 = 0.007854(10-6 ) m2 From Table 4.3, r = 1.7 x 10-8 Ω-m2 /m
22. 22. Solutions for Fundamentals of Modern Manufacturing, 4/e (published by Wiley)  MPGroover 2010 03-03-09, 03-03-09 Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful. 4 R = (1.7 x 10-8 Ω-m2 /m)(10 m)/( 0.007854(10-6 ) m2 ) = 2164.5(10-2 ) Ω = 21.65 Ω 4.7 A 16 gage nickel wire (0.0508-in diameter) connects a solenoid to a control circuit that is 32.8 ft away. (a) What is the resistance of the wire? Use Table 4.3 as a reference. (b) If a current was passed through the wire, it would heat up. How does this affect the resistance? Solution: (a) L = 32.8 ft = 393.6 in Area A = π(0.0508)2 /4 = 0.00203 in2 R = r (L/A) = 6.8 x 10-8 (39.4)(393.6/0.00203) = 0.520 ohm (b) If a current is passed through the wire causing the wire to heat up, the resistivity of the wire would change. Since nickel is a metal, the resistivity would increase, causing the resistance to increase. This, in turn, would cause slightly more heat to be generated. 4.8 Aluminum wiring was used in many homes in the 1960s due to the high cost of copper at the time. Aluminum wire that was 12 gauge (a measure of cross-sectional area) was rated at 15 A of current. If copper wire of the same gauge were used to replace the aluminum wire, what current should the wire be capable of carrying if all factors except resistivity are considered equal? Assume that the resistance of the wire is the primary factor that determines the current it can carry and the cross- sectional area and length are the same for the aluminum and copper wires. Solution: The area and length are constant between the types of wires. The overall change in resistance is due to the change in resistivity of the materials. From Table 4.3: For Aluminum r = 2.8 x 10-8 For Copper r = 1.7 x 10-8 The resistance will reduce by 1.7x10-8 /2.8x10-8 = 0.61 Since I = E/R and Rcu=0.61(Ral), then Icu = 1/0.61*Ial = 15/0.61= 25 A Note that the code value is actually 20 A due to several factors including heat dissipation and rounding down to the nearest 5 amp value.